Post navigation

Common Tests for Welder Performance Qualification

The purpose of welder performance qualifications is to ensure that the welder can deposit sound welds. There are several tests, both destructive and nondestructive, that are used to evaluate a welder’s ability to deposit good welds. Below are four of the most common test applied for these qualifications:

Visual Inspection (VT)

Visual inspection is the first test performed during performance qualifications. Specific instruction can be found in AWS D1.1 Structural Welding Code – Steel 4.9 Methods of Testing and Acceptance Criteria for WPS Qualifications (same applies to performance qualification). After a fillet weld or groove weld is made, visual examination looks for weld discontinuities such as cracks, craters, excessive reinforcement, weld size, undercut and others. No sense is performing destructive testing if performance fails initial visual inspection of the weld.

Bend Test

Bend tests are specific to groove welds. They can either be side, root or face bends. This type of testing is ensuring soundness of the weld. The goal is to have no discontinuities on the bent surface, although most codes have allowances for certain types of discontinuities. After the parts are bent, VT is performed and all discontinuities are measured and then compared to maximum allowed values.

Root and face bend tests for a 2G GMAW test

Macroetch Test

A macroetch test is done to evaluate if the welder achieved fusion to the root of the joint as well as the side walls. This is only required on fillet welds as bend tests would reveal any problems associated with lack of fusion on groove welds. The macroetch can be measured so we know other important values such as depth of penetration at the root and sides. AWS D1.1 requires fusion to the root but not necessarily beyond. This is a useful test, but has one important limitation: you are evaluating fusion and penetration at one specific spot. Cut the part an eighth of an inch to either side and you may have different results. To compensate for this, fillet break tests are performed.

A macroetch tests can reveal lack of root fusion which is not acceptable in welder performance qualification for fillet welds.

Fillet Break Tests

In a fillet break test a section of the joint is cut out, usually about 4 inches in length. The specimen is then placed on a vise or a press and the root of the joint is placed under tension until the part breaks or folds over itself. The break is then examined to assure that there was fusion to the root.

A fillet break test reveals if root fusion was achieve over a specific length of weld.

Codes allow for the use of radiographic testing (RT) in lieu of bend tests in some cases. Additionally, depending on what standard you are following you may be able to use other testing methods such as ultrasonic testing (UT) and leak testing (LT). As always, know the code or standard you are working with as it will provide all the necessary information regarding the tests needed for performance qualification.

Disclosure of Material Connection: Some of the links in the post above are “affiliate links.” This means if you click on the link and purchase the item, we will receive an affiliate commission. Regardless, we only recommend products or services we use personally and believe will add value to our readers. I am disclosing this in accordance with the Federal Trade Commission’s 16 CFR, Part 255: “Guides Concerning the Use of Endorsements and Testimonials in Advertising.”